An Investigation of Abrasion Resistance Property of
Clay- Epoxy Nanocomposite Coating
MUKESH K. MADHUP*1
, NISHA K. SHAH2
and NEHA R. PAREKH2
13M India Ltd, Moraiya Industrial Area, Ahmedabad, Gujarat 382213, India. 2Department of Chemistry, School of Sciences, Gujarat University, Navrangpura
Ahmedabad, Gujarat 380009, India.
Diglycidyl ether of bisphenolA based epoxy resin was loaded with alkyl quaternary ammonium modified bentonite clay nanoparticles (b-CNPs) in various concentrations. The abrasion resistance (Taber) property of the composite coatings cured with amine were investigated after 7 and 60 days curing at two different cycles viz. 500 and 1000. The mass losses of the materials revealed the fact that abrasion resistance increases with increase in CNPs concentration inside epoxy matrix with ageing. Thermal (DSC), spectroscopic (FTIR) and morphological (SEM) studies were performed to characterize the developed epoxy nanocomposite (ENC) coating. A gradual decrease in glass transition temperature (Tg) was observed with increase in the b-CNPs concentration. The modified b-CNPs found interacting with epoxy matrix and the intensity found increasing with increase in b-CNPs concentration during spectroscopic study. Smooth film morphology was revealed by scanning electron microscopic analysis confirming the uniform dispersion of b-CNPs inside polymer nanocomposite matrix.
Received: 03 March 2018 Accepted: 08 May 2018
Epoxy, Nanocomposite, Abrasion, Scanning electron microscopy, Glass transition temperature.
Material Science Research India
CONTACT Mukesh K. Madhup firstname.lastname@example.org 3M India Ltd, Moraiya Industrial Area, Ahmedabad, Gujarat 382213, India.
© 2018 The Author(s). Published by Oriental Scientific Publishing Company
This is an Open Access article licensed under a Creative Commons license: Attribution 4.0 International (CC-BY). Doi: http://dx.doi.org/10.13005/msri/150209
Organic inorganic hybrid nanocomposites show enhanced protective proper ties such as improvements in mechanical1,2, thermal3,4, optical5,6,
electrical7 and magnetic properties8. Polymer clay
nanocomposites are material which consists of polymer as matrix and clay nanoparticles as the
reinforcement fillers9. Improved thermal, mechanical
(strength, modulus, toughness) and physical (barrier) properties over pure nylon matrix were observed during initial research10. Organically
the barrier properties and corrosion protection by incorporation of SiO2, Zn, Fe2O3, halloysite clay nanomaterials were observed in epoxy coating12,13.
The novel polymer electrolyte nanocomposite composed of poly(ethylene oxide), lithium triflate and mineral clay study demonstrated that the addition of optimum content of D-2000 modified montmorillonite increased ionic conductivity of the PEO based electrolyte by nearly 16 times compared
to plain (PEO)8 LiCF3SO3 14. Small improvement
in the anticorrosion properties for the exfoliated SC18/Epon 828/D400 nanocomposite coatings was observed, however there were no improvement for the intercalated organoclay/Epon 828/Y-60 nanocomposite. This result might be related to the better dispersion of silicate nanosheet in the epoxy
matrix for SC18/Epon 828/D400 nanocomposite15.
The processing and chemical characterization of amine cured epoxy/clay nanocompositesby FTIR and FT-Raman methods confirmed that the sonication processing in acetone did not induce chemical changes in the epoxy network. The intercalation of the epoxy network between the clay nanolayers was indicated by the broader tan δ curve observed by DMA. The Tg linearly increased with the increase of the amount of clay nanoplatelets in the amine-cured epoxy matrix16. The incorporation of
organoclay to rubbery and glassy epoxy matrices led to promising mechanical properties improvements even in the absence of additional shear to disperse the clay. With the use of organoclay, an interesting stiffness/toughness balance of nanocomposite for very low filler contents and without reduction in the Tg of the matrix was obtained.17 An advanced
anticorrosive materials were prepared from amine-capped aniline trimer-based electroactive polyimide-clay nanocomposite materials with synergistic effects of redox catalytic capability and gas barrier properties18. Solvent assistance and curing at
elevated temperature are main parameters for clay nanoparticles intercalation. Addition of small amounts of spherical nanoparticles with sufficient hardness such as zirconia nanoparticles assist the exfoliation process due to the shear implying media in nano-scale and fascinates the restoration of the physical and mechanical properties. Mechanical properties of nanocomposites containing various combination of clay and ZrO2 nanoparticles were slightly decreased compared with neat epoxy coating, This phenomena is as a result of formation of nano-sized voids in the
trapped regions by clay stacks, and development of physical barrier clay stacks, which leads to disturb curing procedure and decrease polymer cross linking density. The barrier properties of the nanocomposites increased with the addition of spherical nanoparticles to clay nanocomposites due to better exfoliation process19. Various combination
of epoxy-based nanocomposite coatings containing aminopropyltrimethoxysilane, APS, treated zirconia and clay nanoparticles via slurry method were prepared. It was found that the simultaneous addition of layered clay and small amounts of spherical APS-treated zirconia nanoparticles with sufficient hardness to epoxy coatings significantly improves the corrosion resistance of the nanocomposite coatings.20 Epoxy coating modified by PANI/
clay nanocomposite particles exhibited improved anticorrosion performance in comparison with neat epoxy and epoxy/PANI samples. Furthermore, the corrosion protection efficiency of steel panel coated with epoxy/PANI/OMMT (organo-modified montmorillonite) appeared to be much higher than that of epoxy/PANI/MMT one21. The effects
of different interface strength were significant on the morphology and structure of epoxy/clay nanocomposites. The XRD and SEM analyses proved that the chemical reaction of amino-groups of Jeffamine XTJ502-clay with epoxy created a better interface, resulting in significant mechanical properties enhancement22. The increase in enthalpy
of curing reaction and decrease in peak temperature of nanocomposite corroborated the catalytic effect of clay on the curing process. TEM and X-ray diffraction analysis confirmed both intercalated and exfoliated clay platelet within the epoxy blend23. Two
different procedures were used for the clay mineral dispersion: (i) organically modified montmorillonite (OMt) was dispersed in an epoxy matrix previously modified with acrylate polymers or (ii) the clay mineral was swollen in the acrylate monomers and the monomer was in situ polymerized followed by dispersion in the epoxy matrix. The later procedure provided higher degree of intercalation as indicated by small angle x-ray scattering (SAXS) and transmission electron microscopic (TEM) analysis. TEM microscopy was a very useful tool and indicated the presence of exfoliated/intercalated structures and some aggregates24. The epoxy acrylate-clay
acrylic acid in the presence of clay. The increase in surface hardness was observed which was found in agreement with the increase in glass transition temperature of the nanocomposite films25. A new
type of tetraglycidyl 1, 4′-bis (4-amine-phenoxy) benzene (TGBAPB) epoxy resin containing ether linkage was blended with conventional diglycidyl ether of bisphenol A (DGEBA) epoxy resin in order to overcome the deficient properties that prevented the use of DGEBA for high performance applications. Furthermore, organically modified montmorillonitenano clay of different weight percentages viz. 1%, 3% and 5% were reinforced with the TGBAPB/DGEBA blend epoxy to study its nano reinforcing effect. It was observed that thermal stability, mechanical properties, toughness and stiffness for the TGBAPB/DGEBA blend epoxy and nanocomposites are higher than that of neat DGEBA26.
Automotive, oil & gas pipelines, floorings etc. are important application segments for abrasion resistant polymeric linings as coating. In this article, we report abrasion resistance study of bentonite clay nanoparticles(b-CNPs)/ epoxy nanocomposite (ENC) coating with two different cure time intervals
viz. one after 7 days and other after 60 days and compared it with neat epoxy (unfilled) coating.
Materials and Methods
The clay nanoparticles (CNPs) in the current study is a methyl, tallow, bis 2-hydroxyethyl, quaternary ammonium modified bentonite having diffraction d-spacing (d) 18.5Å, obtained from BYK-Chemie GmbH, Germany commercially known as Cloisite 30B (chemical structure of the organic modifier is illustrated in Fig.1). Diglycidyl ether of bisphenol A (DGEBA) based unmodified medium viscosity liquid epoxy resin Araldite GY-250 obtained from Huntsman Corporation was used as polymer matrix. Amine curative used for crosslinking with epoxy is an aliphatic polyamine commercially known as Ancamine 1856, obtained from Air products, USA. A silicon based surface wetting additive (BASF) was added in small quantity (0.01%) in the coating formulation for surface tension reduction and smooth film formation. The epoxy resin, b-CNPs and surface additives were synthesized as ‘component A’ while
aliphatic polyamine was used as ‘component B’ of the coating system. The Diglycidyl ether of bisphenolAepoxy polymer under study is having epoxide equivalent of 189 g/eq and viscosity of 12,000 cPs at 25°C while the curing agent used is having amine value 460 mg KOH/g and viscosity of 3000 Cps at 25°C.
Synthesis of Clay Epoxy Nanocomposite (ENC) Coating
A 250 ml steel vessel was cleaned and dehydrated for 10 min in oven at 105°C. The vessel was charged with weighed quantity of Diglycidyl ether of bisphenol A epoxy polymer followed by silicon based wetting additive (0.01% by weight of total epoxy resin) and mixed for 5 minutes under mechanical stirrer (Dispermill, ATP Engineering B.V.). In this mixture, b-CNPs were charged to obtain hybrid nanoclay epoxy matrix composition in various desired concentration. A total of six hybrid epoxy matrix were synthesized following this method having weight concentrations 0.12%, 0.25%, 0.5%, 0.75%, 1% and 5% by high speed mechanical dispersion (HSD) method. The dispersion operations were performed at 1000 rpm, 30 minutes each batch following identical process of addition and similar dispersion level. Different dispersion methods have different effect on the clay modified polymers and non-identical dispersion may lead to different thermal, mechanical and performance properties27. Maximum
temperature recorded during the dispersion process was 45°C generated due to frictional force. Entire operation was performed at laboratory conditions, 23+/-1°C temperature and 55% relative humidity (RH).
Clay Epoxy Nanocomposites (ENC) Coating Properties and Concentrations
Various properties were studied at different concentrations of Diglycidyl ether of bisphenol A based epoxy clay nanocomposite coatings. Glass transition temperatures (Tg) and Fourier transform infrared spectroscopy (FTIR) tests were studied for 0% -5.0% CNPs concentrations. Scanning electron microscopy (SEM) were conducted for CNPs as such and ENC at 1% concentration to investigate the surface morphology. Abrasion resistance of the ENC were studied for 0% (neat) - 1.0% concentrations.
Organic–Inorganic Hybrid Nanocomposite Film Preparation
Thin films of epoxy CNPs formulation (component A) were prepared by spray and drawdown methods for various analyses and testing, after mixing in the ratio of 100:40 by weight with polyamine curative (component B). For abrasion resistance studies nanocomposite coatings were applied following gravity feed air assisted spray method on mild steel metal coupons of 100 mm x 100 mm x 1 mm dimension, using Devilbliss spray gun having 1.4 mm nozzle orifice. Abrasion resistance study for various concentrations were performed at 35 (±2) µ-meter dry film thickness (DFT). Before coating applications on mild steel coupons, the surfaces were prepared using emery paper of 180# followed by washing with acetone. Free films for scanning electron microscopy (SEM) analysis were prepared by draw down method on silicon release paper with calculated amount of material to have 25 µ-meter uniform dry film thicknesses. The applied films were kept at 23°C for 7 days before subjecting for test. Draw downed, dried composite films were used for thermal and spectroscopic studies.
Instrumental Characterization and Performance Testing
Different set of analyses and abrasion resistance property were studied for various concentrations of b-CNPs-ENC coatings. Thin films of clay doped Diglycidyl ether of bisphenol A Epoxy coating materials were prepared by spray and drawdown methods for various analyses and testing. The abrasion resistance test of Cloisite®30B-Epoxy composite coatings was carried out according to ASTM D4060-01 method, for 0% (n-E), 0.12%, 0.25%, 0.5%, 0.75% and 1.0% concentrations. The
carbon steel coupon surfaces were prepared using 3M aluminum oxide emery paper, 180# followed by washing with acetone before coating. The applied coatings/films were conditioned at 23°C for 7 days before testing. Draw downed, dried coating films were used for thermal and spectroscopic studies.
The thermal properties of the films were measured using differential scanning calorimetry (DSC) of TA Instruments, Inc. The weights of the samples were taken 10 milligrams each for thermal study of the composite coating. The glass transition temperature (Tg) of hybrid nanocomposite samples were measured heating from 25 to 200oC at a heating
rate of 20oC/min under nitrogen atmosphere at a flow
rate of 30 mL/min. The abrasion resistance test was carried out according to ASTM D4060-01 method. Scanning electron microscope (SEM) of JEOL-Tokyo model JSM-6510 LV was used to characterize the surface morphology of CNPs and ENCs film. Fourier transform infrared (FTIR) spectroscopic studies were done to investigate the interaction of b-CNPs with epoxy amine system in different concentrations using Thermoscientific Nicolet i-S10 instrument. Film applications for various types of specimen preparation under study were done by spray gun (Devilbliss, 1.4mm nozzle orifice) and draw down methods. The dry film thicknesses (DFT) of the films were measured by Elcometer - 456 thickness gauge.
Results and Discussions
Spectroscopic (FTIR) Studies of Cloisite®30 B-ENC Composite Film
Fourier transform infrared spectroscopy (FTIR) method was adopted to confirm the changes in the chemical structures of the composite materials. To examine the possible interaction between the clay nano material and Diglycidyl ether of bisphenol A Epoxy, a series of FTIR studies were carried out for various concentrations of b-CNPs-ENC coatings. The spectroscopic analysis was performed to analyze neat epoxy (n-E) and various concentrations of the epoxy polyamine nanocomposite coatings. The cured Cloisite®30B-epoxy polyamine nanocomposite (b-CNP-ENC)films were crushed to powder for this analysis. To closely visualize the spectral changes the spectra between 400 cm-1 to 2500 cm-1 are plotted
are observed in the range between 4000 cm-1 &
400 cm-1. The first one, at 915 cm-1, is attributed to
the C-O deformation of the oxirane group, and the second band is located at 3050 cm-1 approximately
and is attributed to the C-H tension of the methylene group of the epoxy ring. This band is not very useful since its intensity is low and it is also very close to the strong O-H absorptions; but in low polymerization degree epoxy monomers it can be used as a qualitative indicative of the presence of epoxy
groups.The peaks were observed at 3400 cm-1 for
–OH group (moisture), 2360 cm-1 for carbon dioxide,
1635 cm-1 for –OH, 1384 cm-1 for CO
32- and 1170
an enlarged portion of wavenumbers between 400 cm-1 to 1000 cm-1 has been plotted to distinctly
visualize the spectral differences (Fig.3). Gradual enhancement in chemical interaction was observed with increase in Cloisite®30B concentration from 0.12% to 5%as corroborated by the peak intensity.A prominent peak was observed at wavenumber 462 cm-1 which shows interaction or inclusion of b-CNPs
inside matrix of epoxy amine system. Different stretching/bending vibrations of chemical moieties in the infrared spectraobserved during neat epoxy (0%) and epoxy NCCs have been given in Table 1.Two characteristic absorptions of the oxiranering
Fig. 2: FTIR scans of various concentration of Cloisite®30B doped nano-composite coating between 400 cm-1 to 2500 cm-1.
Fig.3: FTIR scans between 400 cm-1 to 1000 cm-1 to illustrate the interaction of Cloisite-30B with epoxy polyamine matrix; with increasing concentrations of Cloisite 30 B, a new
cm-1 for C-O. There are also bands corresponding to
the ether linkage located at 1000-1100 cm-1 28. It is
noteworthy that b-CNPs are interacting with epoxy polyamine system and the intensity of the peaks at 462 cm-1 has been increasing with increase in
concentration of Closite®30B from 0.12% to 5% concentrations. The initial interaction of the organo-clay with epoxy polyamine matrix is visible at 0.12% concentration with minor change in peak position and shift in peak intensity compared to n-E (0%). The changes at 0.25% concentration remained almost similar to the 0.12% concentration, a distinct peak of b-CNPs interaction appeared. Similar interaction with slightly increased intensity is visible at 0.75% and 1% concentrations. A very broad peak appeared with increase in concentration at 5% concentration which signifies the presence of Clositie®30B in the formulation.
Morphological (SEM) Characterization of b-CNPs-ENC Film
The surface morphologies at various magnifications and scales of Cloisite®30B doped nanocomposite(b-CNPs-ENC) coating at 1.0% concentration are illustrated in Fig.4.1 A, B and C for 40x, 200x and 400x magnifications respectively. It is evident from the SEM images of b-CNPs-epoxy NCCs film that the clay particles are completely dispersed inside Diglycidyl ether of bisphenol A Epoxy matrix with very smooth surface on top. This type of film
Fig. 4. 2: Enlarged view of undispersed particles visualized in SEM image Fig. 4.1.B with measured particle size Fig. 4. 1: SEM scan of Cloisite®30B-ENC,
1% concentration at 40x. [A]; 200x [B]; 400x [C], smooth surface finish, few bigger
agglomerates distinctly visible at surface. Table 1: Spectral vibrations of different
groups present in b-CNPs-ENC
Groups present Wavenumber (cm-1)
b-CNPs interaction inside 462
-CH, -NH Bend 557
-AR=C-H, C-H Bending out 754
of plane (polyamide adduct)
1, 4- substitution of epoxy 828
-C-O-R Ether 1035
-C-N absorption of amine 1105
-C-N absorption of amine 1182
Aromatic -C=C- H Vibration 1457
Aromatic -C=C- H Vibration 1508
Aromatic -C=C- H Vibration 1608
smoothness which signifies uniformity in clay dispersion is expected to yield extremely high level of barrier property.
A few agglomerate of clay clusters measuring approximately 18, 21, 25, 23, 29 and 31 µ-meters are also visible on the surface, it is more distinctly visible in Fig.4.B. An enlarged view of the agglomerate has been shown in Fig.4.2 to distinctly visualize the agglomerate particles and their size. The reason of appearance of agglomeratemight be attributed to the undispersed particles during mechanical dispersion process ofb-CNPs inside Diglycidyl ether of bisphenolAepoxy matrix. The surface is smooth with no surface cracks, protrusion or non-uniformity visible in Fig.4.1.C. At 400x magnification, a few very small spread of b-CNPs are visible protruded from surface.
Thermal (DSC) Characterization of Bentonite -ENC Films
The glass transition temperature (Tg) of neat epoxy (n-E, 0%) and epoxynanocomposite coatings (NCCs) in various concentrations viz. 0.12%, 0.5%,
1.0% and 5.0% were determined using differential scanning calorimeter (DSC) of TA Instrument model Q-20.The overlay of thermograms analyzed for various concentrations are given in Fig.5. The Tg is found to be shifting towards lower temperatures with increase in concentration of Cloisite®30B inside Diglycidyl ether of bisphenol A epoxy matrix observed in the thermogram. The lowering in the Tg of Diglycidyl ether of bisphenol A Epoxy NCCs can be attributed to the non-cross linking with amine due to masking of reactive oxirane group by clay nanolayers inside polymer matrix. The lowering in Tg of nanocomposites has also been reported earlier in epoxy clay study by DSC analysis29 and by solid state
NMR study30. The glass transition temperature of the
bentonite clay epoxy nanocomposite coating studied here in general, gradually decreasing with increase in clay material inside the epoxy matrix. It can be observed that at 0.12% and 0.50% concentration, there is almost negligible reduction in Tg while in case of 1% and 5% concentrations there is minor reduction when compared with neat epoxy coating, listed in Table.2.
Fig. 5: Overlay of thermograms of neat epoxy (n-E) and Cloisite®30B-Epoxy nanocomposite coatings, Tg of the nanocomposite decreases with increase in Cloisite® 30B concentration.
Table 2: The glass transition temperature of b-CNPs-ENC
Cloisite 30B (b-CNP) concentration 0 0.0012 0.005 0.01 0.05
Fig. 6: Plot of mass loss of ENCs versus concentration of bentonite clay (b-CNPs) for abrasion resistance test at CS-17 wheel, 1Kg load, after 7 days as per ASTM D4060.
A. mass loss data with increase in concentration of nanoclay after 500 cycles
Fig.7: Plot of mass loss of ENCs versus concentration of bentonite clay (b-CNPs) for abrasion resistance test at CS-17 wheel, 1Kg load, after 7 days as per ASTM D4060,
mass loss data with increase in concentration of nanoclay after 1000 cycles.
Fig. 9: Plot of mass loss, after 60 days at 1000 cycles
Fig. 10: Comparative mass loss after 7 & 60 days cure, 500 cycles.
The finding on Tg in current research is supported by earlier research works that a slight increase or almost no change in Tg occurs in the systems with the organically treated clays modified by surfactants that bears polar group (-OH groups etc.)31,32,33,34. In
those cases, where stronger interaction happens due to hydrogen bond between modifiers and epoxy, it might restrict the motion of epoxy network to some extent which in turn may result into higher Tg. The data of Tg states that in current system of b-CNPs-ENC coating, the nanolayers have not affected the thermal properties much upto 0.5% concentration, while at 1 and 5% concentrations, there might be minor reduction in crosslink density due to masking of reactive epoxide group of the coating making it softer hence, reduction in Tg.
Abrasion Resistance of cloisite®30B-ENC Coating
The abrasion resistance test of the Cloisite30-Epoxy nanocomposite coatings were performed using Taber abrasion test method. The Taber abrasion test is used for the determination of the resistance of organic coatings to abrasion produced by the Taber Abraser on coatings applied to a metal panel. In current research work, the abrasion resistance values of nanocomposite coatings were determined by weight loss calculation method (method B) of
the ASTM D4060 method35. Abrasion resistance is
calculated as loss in weight at a specified number of abrasion cycles, as loss in weight per cycle, or as number of cycles required to remove a unit amount of coating thickness.
Two different sets of specimen were prepared simultaneously using same material and similar application process for abrasion resistance study of b-CNPs-ENC coating. Coated specimen were tested at different time intervals to understand the effect of clay nanolayers inside Diglycidyl ether of bisphenol A epoxy matrix with cure time. The first set of experiment was performed after 7 days and that of second set after 60 days of curing. Both studies were performed after conditioning the test specimen in similar laboratory conditionat 23+/-2˚C temperature and 55% relative humidity (RH).
Abrasion Resistance of b-CNPs-ENC Coating after 7 Days Curing
The abrasion resistance test conducted on 7 days cured film revealed that the Diglycidyl ether of bisphenol A epoxy -polyamine coating in unfilled condition (n-E, 0%) loses higher mass compared to Cloisite®30Bdoped ENC coating. Surprisingly, with mere introduction of b-CNPs at 0.12% concentration, the coating material demonstrated great enhancement in abrasion resistance property. The mass loss data for 7 days cured composites are plotted in Fig.6 and Fig.7 after 500 and 1000 cycles respectively. The best result was observed at 0.12% b-CNPs concentration for both the cycles.
It is noteworthy that the abrasion resistance result of 1% b-CNPs concentration observed a little poorer compared to n-E. The phenomena of improvement in abrasion resistance of the Diglycidyl ether of bisphenol A epoxy polyamine matrix with the introduction of bentonite clay might be attributed to higher compactness of the film due to clay filled Diglycidyl ether of bisphenol A epoxy, interaction of organically modified clay with Diglycidyl ether of bisphenol A epoxy amine matrix (reveled during FTIR study), shape and size of the clay particles and dispersion of particles inside the matrix. When compared among various concentrations, the higher abrasion resistance observed at lower concentration while gradual increase in concentration reduced the abrasion resistance from 0.25 to 1% concentration corroborates that with increase in the clay nanolayers inside matrix the bonding between organicmoiety and inorganic clay decreased when cured for a limited period upto 7 days.
Abrasion Resistance b-CNPs-ENC Coating after 60 Days Curing
that the mass loss has decreased from 29.6 mg to 18.2 mg when tested to n-E and concentration of b-CNPs increased to 0.75% after 60 days exposure for 500 cycles. The decrease in mass loss compared to 7 days with extended curing period of 60 days indicates that the rigidity of the b-CNPs-ENC coating system has increased with time with increase in concentrations. Similarly, the specimen tested for 1000 cycles depicted least abrasion resistance at 0% (n-E) concentration, which got enhanced with b-CNPs doping. The mass loss reported for n-E is 53.3 mg while for 0.75% concentration it is 28.1 mg. The trend after complete cure is in agreement with FTIR interactions where gradual increase in peak observed with increasing intensity up to 0.75% concentration and depicted a very broad peak at 1% concentration. A minor decrease in abrasion resistance at 1% concentration shows that the b-CNPs are in excess for interaction with polymeric matrix. This is depicted in the FTIR scan for 1% with appearance of a very broad peak. 0.75% concentration has resulted as best concentration for abrasion resistance in current study.
Comparative Analysis of b-CNPs-ENC Coating, 7 & 60 Days Curing
The comparative results of mass losses of 7 days and 60 days for neat epoxy (n-E, unfilled) depicts that it is having higher resilience in the chain after 7 days cure and illustrated higher abrasion resistance compared to that of tested after ageing for 60 days. The data of two separate cycles (500 and 1000) are plotted to understand how doping of b-CNPs behaves after 7 days and 60 days curing on abrasion resistance property. The plots of comparative mass losses are illustrated in Fig.10 & Fig.11. With introduction of b-CNPs inside Diglycidyl ether of Bisphenol A Epoxy matrix, enhancement observed in abrasion resistance even after 7 days. Also, after ageing 60 days, higher concentrations of b-CNPs have resulted into better resistance against abrasion which was not the case when tested after 7 days (0.12% performed best). It also implies that with time, the b-CNPs based nanocomposite film becomes more difficult to abrade out compared to neat Diglycidyl ether of Bisphenol A Epoxy. The enhancement in the abrasion resistance property can be attributed to gradual increase in the molecular interactions, film compactness due to inorganic b-CNPs filled inside matrix and lower movement in chain (higher rigidity) when completely
cured thereby making it tougher for abrasion. It is also a resultant of interaction of clay particles with polymer matrix observed in FTIR analysis and platy shape with good dispersion inside Diglycidyl ether of bisphenol A epoxy matrix revealed by SEM analysis during current study. Higher interaction of clay nanoparticles for the properties improvements is in agreement with the earlier work reported by Jena KK, et al36. Also, the decrease in mass loss
with increase in the concentration of b-CNPs has been reported due to increase of inorganic materials inside polymer matrix37.
During current study it is noticed that approximately 0.75% concentration of modified bentonite CNPs (Cloisite 30B) is optimum for improvement and retention of abrasion resistance property of the currently designed coating system with time. The higher abrasion resistance coating so developed based on epoxy clay nanocomposite can have novel applications in various protective coatings systems including home and industrial floors (highly abusive area where conventional coatings show limited protection), mild steel pipes (wear happens during transportation), automotive engineering appliances etc. which undergo wear and tear with time.
depicted important contribution in enhancement of the abrasion resistance properties achieved. The improved abrasion resistance coating developed with incorporation of bentonite clay nano-particles can be applied for the protection of floors, pipes, automotive appliances etc.
The corresponding author, Mukesh Kumar Madhup would like to acknowledge his employer 3M India
Ltd. for providing permission for perusal of doctoral research at Gujarat University, Ahmedabad. Also, he is thankful to Dr. Sridhar Krishnamurthy, Mr. Abhijeet A. Saungikar, Mr. T. H. Venkatesh and Mr. Vijay G. Pillai for their continuous encouragement and support for higher study.
Conflict of Interest
The author(s) declare(s) that there is no conflict of interests regarding the publication of this article.
1. Wetzel B, Haupert F, Qiu Zhang M. Epoxy nanocomposites with high mechanical and tribological performance; Composites Science and Technology 2003; 63 (14): 2055-2067.
2. Mian Wang, Xiaosha Fan, WarintornThitsartarn, Chaobin H. Rheological and mechanical properties of epoxy/clay nanocomposites with enhanced tensile and fracture toughnesses;
Polymer 58 (2015) 43-52.
3. Zheng K, Chen L, Li Y, Cui P. Preparation and
thermal properties of silica-graft
acrylonitrile-butadiene-styrene nanocomposites. Polymer
Engineering & Science 2004; 44 (6):1077-1082.
4. Sushanta K. Sahoo, SmitaMohanty, Sanjay
K. Nayak. Study of thermal stability and thermo-mechanical behavior of functionalized soybean oil modified toughened epoxy/
organoclaynanocomposite; Progress in
Organic Coatings 88 (2015) 263–271.
5. Caseri W. Nanocomposites of polymers
and metals or semiconductors: Historical background and optical proper ties;
Macromolecular Rapid Communications
2000; 21(11): 705-722.
6. Li H, Wang D, Fan H, Wang P, Jiang T, Xie
T. Synthesis of highly efficient C-doped TiO2 photocatalyst and its photo-generated charge-transfer properties; Journal of Colloid and Interface Science 2011; 354 (1): 175-180.
7. Hu G, Zhao C, Zhang S, Yang M, Wang
Z. Low percolation thresholds of electrical conductivity and rheology in poly(ethylene
terephthalate) through the networks of multi-walled carbon nanotubes; Polymer 2006; 47(1): 480-488.
8. Zhang M, Sun G, Guo D, Jin Z. Improvement
of the magnetic properties of nanocomposite permanent magnetic alloys with Dy and Ga substitutions; Journal of Materials Processing Technology 2002; 120 (1–3): 265-269.
9. Fukushima Y, Okada A, Kawasumi M,
Kurauchi T, Kamigaito O. Swelling behaviour of montmorillonite by poly-6-amide; Clay Minerals 1988; 23 (1): 27-34.
10. Usuki A, Kojima Y, Kawasumi M, Okada A,
Fukushima Y, Kurauchi T, et al. Synthesis of nylon 6-clay hybrid; Journal of Materials Research 1993; 8 (05): 1179-1184.
11. S . S . R a y, M . O k a m o t o . Po l y m e r / layeredsilicatenanocomposites: a review from preparation to processing; Prog.Polym. Sci. 28 (11) (2003) 1539–1641.
12. Mei-Chun Lai, Kung-Chin Chang, Jui-Ming
Yeh, Shir-Joe Liou, Ming-FaHsieh,Herng-Show Chang. Advanced environmentally friendly anticorrosive materials prepared from water-based polyacrylate/Na+-MMT clay nanocomposite latexes; Eur. Polym. J. 43 (10) (2007) 4219–4228.
13. Xianming Shi, Tuan Anh Nguyen, ZhiyongSuo,
Yajun Liu, RecepAvci. Effect of nanoparticles on the anticorrosion and mechanical properties of epoxy coating; Surf.Coat.Technol. 204 (3) (2009) 237–245.
14. Chen, H.-W., Chang, F.-C..The novel polymer
clay; Polymer; 42 (2001) 9763.
15. C. Chen, M. Khobaib, D. Curliss. Epoxy
layered-silicate nanocomposites; Prog. Org. Coat. 47 (2003) 376.
16. H. Miyagawa, M.J. Rich, L.T. Drzal. Amine-Cured Epoxy/Clay Nanocomposites. I. Processing and Chemical Characterization;
J. PolymSci Part B: Polym Phys., 42 (2004) 4384.
17. Le Pluart L, Duchet J, Sautereau H. Epoxy/
montmorillonitenanocomposites: influence of organophilic treatment on reactivity, morphology and fracture properties; Polymer.; 46(26) (2005) 12267.
18. Huang, Hsiu-Ying ; Huang, Tsao-Cheng ; Yeh,
Tzu-Chun ; Tsai, Chung-Yen ; Lai, Cheng-Ling; Tsai, Mei-Hui; Yeh, Jui-Ming ; Chou, Yi-Chen. Advanced anticorrosive materials prepared from amine-capped aniline trimer-based electroactive polyimide-clay nanocomposite materials with synergistic effects of redox catalytic capability and gas barrier properties;
Polymer; 52(11) (2011) 2391.
19. S.M. Mirabedini, M. Behzadnasab, K.
Kabiri, Effect of various combinations of zirconia and organoclay nanoparticles on mechanical and thermal properties of an epoxy nanocomposite coating; Composites: Part A; 43 (2012) 2095.
20. M. Behzadnasab, S.M. Mirabedini; M.
Esfandeh.Corrosion protection of steel by e p ox y n a n o c o m p o s i t e c o a t i n g s containing various combinations of clay and nanoparticulate zirconia; Corro.Sci.; 75 (2013) 134.
21. Amir H. Navarchian, Mehrnaz Joulazadeh,
Fariba Karimi. Investigation of corrosion p r o t e c t i o n p e r fo r m a n c e o f e p ox y coatingsmodified by polyaniline/clay nanocomposites on steel surfaces; Progress in Organic Coatings; 77 (2014) 347.
22. Izzuddin Zaman, Fethma Nor, Bukhari
Manshoor, Amir Khalid, Sherif Araby. Influence of interface on epoxy/clay nanocomposites: 1. morphology structure;Procedia Manufacturing; 2 (2015) 17.
23. Sushanta K. Sahoo,SmitaMohanty, Sanjay
K. Nayak. Study of thermal stability and thermo-mechanical behavior offunctionalized soybean oil modified toughened epoxy/
organoclaynanocomposite;Prog. Org. Coat.
88 (2015) 263.
24. Adriana A. Silva, Bluma G. Soares, Karim Dahmouche. Organoclay-epoxy nocomposites modified with polyacrylates: The effect of the clay mineral dispersion method; Applied Clay Science; 124–125 (2016) 46–53.
25. A. Dehghan. M.J. Zohuriaan-Mehr, A. Salimi.
Rapid preparation of epoxy acrylate-clay nanocomposite: Simultaneous acrylation/ nanoclay dispersion under ultrasonication;
Prog. Org. Coat.; 108 (2017) 44.
26. DhanapalDuraibabu, DesikanRajagopal,
SrinivasanAnanda Kumara. A first MMT reinforced nanocomposite functionalized with etherlinkage derived from tetraglycidyl/ diglycidyl epoxy building block; Prog. Org. Coat.; 104 (2017) 135.
27. Adriana A. Silva, Bluma G. Soares,
KarimDahmouche. Organoclay-epoxy nocomposites modified with polyacrylates: The effect of the clay mineral dispersion
method; Applied Clay Science 124–125
28. M.K. Madhup, N.K. Shah, P.M. Wadhwani;
Investigation of surface morphology, anti-corrosive and abrasionresistance properties of nickel oxide epoxy nanocomposite (NiO-ENC)coating on mild steel substrate; Progress in Organic Coatings 2015; 80:1–10.
29. Akbari B, Bagheri R. Deformation mechanism
of epoxy/clay nanocomposite; European
Polymer Journal 2007; 43(3):782-788.
30. Zax D, Yang D, Santos R, Hegemann H,
Giannelis H, Manias E. J ChemPhys; 112(6) (2000) 1951-4.
31. Messersmith PB, Giannelis EP. Synthesis and
Characterization of Layered Silicate-Epoxy
Nanocomposites.Chemistry of Materials.
32. Miyagawa H, Rich MJ, Drzal LT. Amine-cured
epoxy/clay nanocomposites. I. Processing and chemical characterization. Journal of Polymer Science Part B: Polymer Physics. 2004;42(23):4384-4390.
33. Liu Z, Erhan SZ, Xu J. Preparation,
characterization and mechanical properties of epoxidized soybean oil/clay nanocomposites.
montmorillonitenanocomposite.Journal of Applied Polymer Science. 2002;86(2):414-421.
35. ASTM D4060-14, Standard Test Method for
Abrasion Resistance of Organic Coatings by the Taber Abraser, ASTM International, West Conshohocken, PA, 2014, www.astm.org.
36. Jena KK, Raju KVSN, Narayan R, Rout
TK. Sodium montmorillonite clay loaded
novel organic–inorganic hybrid composites: Synthesis and characterization; Progress in Organic Coatings. 2012; 75(1–2):33-37.
37. Guo Z, Pereira T, Choi O, Wang Y, Hahn HT.
Surface functionalized alumina nanoparticle filled polymeric nanocomposites with
enhanced mechanical properties; Journal